Int. J. Electrochem. Sci., 13 (2018) 10217 – 10232, doi: 10.20964/2018.11.11
International Journal of
Effect of the Particle Size of 316L Stainless Steel on the
Corrosion Characteristics of the Steel Fabricated by Selective
Wei Chen1, Guangfu Yin1,*, Zhongbing Huang1, Zai Feng2 1
College of Materials Science and Engineering, Sichuan University, Chengdu, 610065, China 2
Sichuan Hengchuang Bolian Technology Co., Ltd, Chengdu, 610044, China *
Received: 10 June 2018 / Accepted: 6 August 2018 / Published: 1 October 2018
The corrosion characteristics of 316L stainless steel (SS316L) fabricated by selective laser melting (SLM) in a 6.0 wt.% FeCl3 solution was investigated in this study. To analyse the relationship between the corrosion factor and powder feedstock, three samples were made by SLM with three particle sizes, and their potentiodynamic polarization curve were measured using a CHI660E electrochemical working station in a 6.0 wt.% FeCl3 solution at 25 °C. The microstructure was investigated by optical microscopy (OM) and scanning electron microscopy (SEM). Corrosion products analyses were performed using an X-ray energy dispersion spectroscopy (EDS) detection system. The results showed that the SLM samples prepared with fine powder possessed the best surface quality with a much lower porosity and without un-melted powder particles. Compared with the SLM samples from the coarse powder and raw powder, the SLM samples from fine powder exhibited a higher corrosion potential (Ecorr) by 18.94 %, 28.09 % and 67.33 % at the XY-plane, the XZ-plane and the YZ-plane, respectively. However, the corrosion current density (icorr) at the three cross-sections of the SLM sample from fine powder was not lower than that of the other two samples. The weight loss of the SLM sample from fine powder was the highest. These results indicated that the corrosion tendency of the SLM sample from the fine powder was the lowest, but its corrosion rate was the fastest.
Keywords: selective laser melting; stainless steel; corrosion characteristics; anodic polarization; immersion testing.
this technique, it is possible to manufacture high-accuracy and more complex structural parts that could not be previously produced by traditional manufacturing methods. AM technologies include laminated object manufacturing (LOM) , directed energy deposition (DED) , stereo lithography appearance (SLA) , selective laser sintering (SLS) , selective laser melting (SLM) , electron beam melting (EBM)  and binder jet 3D printing (BJ3DP) . SLM has been one of the most used powder bed AM processes developed for rapid prototyping with metal powders, which can be used to produce metal parts with almost complete density, excellent mechanical properties, high dimensional accuracy, and a high material utilization ratio. A great deal of studies has been performed to establish the relationship among the process, microstructure, defects and mechanical performance for stainless steel , aluminium , nickel , pure tantalum and titanium alloys [11,12]. SLM has attracted the interest of a large number of researchers’ in multiple domains such as the aerospace , nuclear and biomedical industries [11,14].
316L stainless steel (SS316L) is a type of austenitic stainless steel with high corrosion resistance and could be utilized in the medicine and food industries [15-17]. The corrosion resistance of SS316L produced by SLM has been researched. It is generally known that the corrosion resistance of stainless steel is mainly determined by its chemical composition, microstructure and porous defects. These factors are also controlled by the initial SLM processing parameters such as laser power, scanning speed, hatch distance, layer thickness and beam spot diameter. The corrosion characteristics of as-cast and sintered SS316L samples in sulphuric acid and phosphoric acid solution were studied . It was found that compared to cast samples, the sintered samples exhibited a lower corrosion resistance in both solutions due to the presence of residual pores in the microstructure. The effect of the porosity on the corrosion behaviour of hot-pressed stainless steel (HPSS) in sulphuric acid was investigated . The results showed that the porosity of HPSS was the major factor affecting its corrosion resistance. The high porosity led to a low corrosion resistance. It was shown that the primary mechanism that affected the corrosion resistance of HPSS in a H2SO4 solution was the evolution of the hydrogen concentration cell produced by the electrolysis stall in the communication open cell. Thus, the exposed cell surface during communication served as an active anode, and the surface of the engineering sample acted as an active cathode. The relationship between surface quality and corrosion resistance of the SLM SS316L sample was inspected . The results indicate that high surface quality could enhance the corrosion resistance of the SS316L parts manufactured via SLM. The corrosion behaviour of grade SS316L fabricated using casting, hot isostatic pressing (HIP), SLM and SLM + HIP in H2SO4 solution was examined . The electrochemical results showed that the manufacturing method had a significant effect on the corrosion resistance of SS316L parts. The effect of the powder size distribution on the sintering kinetics along with empirical models for solid-state and supersolidus liquid phase sintering (SLPS) of Inconel 718 parts fabricated by BJ3DP was discussed . The results indicated that the powder size distribution affected the properties of the 3D printed parts.
with three particle sizes were used to investigate the relationship between the particle size and corrosion characteristics in a 6.0 wt.% FeCl3 solution.
2. EXPERIMENTAL PROCEDURE
2.1. SS316L powder
The SS316L spherical powder was prepared by a gas atomization process with the following parameters: an atomization temperature of 1550-1600 °C, a liquid-metal flow velocity of 10 kg/min, and an inlet nitrogen gas pressure of 6.0 MPa. Mesh sieving and cyclone separation were used to select the three kinds of SS316L powders with a median particle size (d50) of 8.29 μm (fine powder), 20.31 μm (coarse powder) and 14.63 μm (raw powder) with a composition of Cr 17.42 wt.%, Ni 11.61 wt.%, Mo 2.27 wt.%, Mn 1.49 wt.%, Si 0.75 wt.%, C 0.019 wt.%, P 0.008 wt.%, S 0.003 wt.%, O 0.005 wt.% and the balance Fe for SLM processing. The microstructure of the three sizes of the SS316L powders was presented in Figure 1, which shows a highly spherical shape suitable for the SLM process.
Figure 1. SEM morphologies of three SS316L raw powder (a), coarse powder (b) and fine powder (c).
2.2. Selective laser melting (SLM)
The metallic parts were manufactured using the SLM process by the AFS-M120 (Longyuan AFS Co. Beijing, China). The processing parameters were as follows: maximum laser power of 500 W, laser spot diameter of 70 μm, hatch distance of 60 μm, scanning speed of 2000 mm/s and layer thickness of 30 μm. The schematic diagram of laser scanning path strategy is shown in Figure 2. The XY-plane was the scanning direction, and the YZ-plane and XZ-plane were the building directions.
2.3. Electrochemical tests
The potentiodynamic polarization curves were measured using a CHI660E electrochemical working station at 25 °C in a 6.0 wt.% FeCl3 solution. The test cell included a saturated calomel electrode as the reference electrode, a platinum counter electrode, and the SS316L SLM sample as the working electrode. The working electrode was embedded in epoxy resin with only an exposed area of 0.25 cm2 that remained for testing. The polarization curves were swept at a scan rate of 1 mV/s from an initial potential of -1.0 V to a final potential of 1.2 V  and started after a 30 min immersion of the samples in a 6.0 wt.% FeCl3 solution. Three independent trials were conducted under the same conditions.
2.4. Immersion corrosion experiment
In the immersion corrosion tests, the square-shaped samples were polished using SiC paper from 320 grit down to 2000 grit. The samples were cleaned with ethanol and the initial weight as well as the dimensions of the samples was measured. The samples were then immersed in a 6.0 wt.% FeCl3 solution. The samples were removed from the solution every 24 h, then washed with distilled water, dried in hot air and then weighed by an analytical balance (Zhuojing Co. Shanghai, China) with the smallest increment of 0.1 mg. The samples were then re-immersed in the FeCl3 solution again for 24 h. The corrosion products were not deliberately removed at any intermediate stages but were removed only after the last analysis for microscopic investigations. Three independent trials were conducted under the same conditions after a time period of 1, 2, 3, …, 25 days.
corrosion products was measured by X-ray diffraction (XRD, D8 Advance, Bruker, Germany) with Cu-Kα radiation with a wavelength of 1.5405 Å at 40 kV and 40 mA in the 2-theta range 0-90° at a scan rate of 0.05°/s.
3. RESULTS AND DISCUSSION
3.1. Potentiodynamic polarization curves
Figure 3 shows the potentiodynamic polarization curves of the three SS316L SLM samples. It could be seen that there was no passivation platform on the potentiodynamic polarization curves. Electrochemical parameters including the corrosion potential (Ecorr), the corrosion current density (icorr), the cathodic Tafel slope (bc) and the anodic Tafel slope (ba) were calculated by Tafel extrapolation from Figure 3, and the results are shown in Table 1. These parameters are normally used to represent the active dissolution of the materials in the form of Ecorr and icorr . The Ecorr of the SS316L SLM samples from coarse powder and raw powder at the XY-plane were 0.095 V and 0.096 V, at the XZ-plane were 0.089 V and 0.093 V, and at the YZ-plane were 0.101 V and 0.098 V, respectively. The Ecorr of the SS316L SLM samples from fine powder was higher than that from coarse powder and raw powder at three planes. The Ecorr of the SS316L SLM samples from coarse powder and raw powder was similar at the three planes. Additionally, the icorr data indicated that the SS316L SLM fine powder YZ-plane sample exhibited the highest icorr (approximately 38.68 μA/cm2).
Figure 3. Polarization curves of the SS316L SLM samples’ XY-Plane (a), XZ-Plane (b) and YZ-Plane (c) in a 6.0 wt.% FeCl3 solution at 25 °C.
Table 1. Electrochemical parameters of three SS316L SLM samples in the 6.0 wt.% FeCl3 solution at 25 °C.
Specimens Ecorr [V] icorr [μA/cm2] -bc [V/dec] ba [V/dec] Fine powder
XY-plane 0.113 17.58 0.07 0.11
XZ-plane 0.114 19.27 0.08 0.10
YZ-plane 0.169 38.68 0.10 0.09
Coarse powder SLM
XY-plane 0.095 16.02 0.07 0.11
XZ-plane 0.089 27.06 0.08 0.12
YZ-plane 0.101 21.49 0.08 0.11
Raw powder SLM Sample
XY-plane 0.096 19.16 0.08 0.13
XZ-plane 0.093 18.45 0.08 0.13
YZ-plane 0.098 18.87 0.07 0.12
However, the icorr at the three cross-sections of the SLM fine powder sample was not lower than that of the other two samples. This result indicated that the corrosion tendency of the SS316L SLM sample from fine powder was the lowest, but its corrosion rate was the fast.
Figure 5. Microstructure of the fine powder XY plane (a), coarse powder XY plane (b), raw powder XY plane (c), fine powder YZ plane (d), coarse powder YZ plane (e), raw powder YZ plane (f), fine powder XZ plane (g), coarse powder XZ plane (h) and raw powder XZ plane (i).
As shown in Figure 4, the morphology of the SS316L SLM samples from different particle size distribution powders exhibited large differences. The SS316L SLM samples from fine powder had the best surface quality which was smoother with less porosity and defects, while the SS316L SLM samples from coarse powder and raw powder had the worst surface quality with vast porosity and defects.
powder was almost completely melted. The contents of the un-melted powders in the SS316L SLM samples from coarse powder and raw powder were the same.
Figure 6. Low magnification of the SEM images of the SLM SS316L samples after anodic polarisation testing in a 6.0 wt.% FeCl3 solution at 25 °C: fine powder XY plane (a), coarse powder XY plane (b), raw powder XY plane (c), fine powder YZ plane (d), coarse powder YZ plane (e), raw powder YZ plane (f), fine powder XZ plane (g), coarse powder XZ plane (h) and raw powder XZ plane (i).
samples from the fine powder. The corrosion could only take place in the holes, pores and microcracks whose potential were high enough . At the same time, the corrosion products dissolved in solution quickly .
Figure 6 shows the low magnification of the SEM images of the nine SLM SS316L samples after anodic polarisation testing in a 6.0 wt.% FeCl3 solution at 25 °C. It could be seen that the corrosion morphology of the nine SLM SS316L samples was similar and the surface of the samples contained a large number of corrosion holes, which is typical pitting corrosion after this type of polarisation test in a 6.0 wt.% FeCl3 solution. From Figure 6, the radius of most pits exceeded 50 μm. SS316L was particularly sensitive to pitting corrosion in the presence of chloride ions . The Cr content of SS316L was high, and a passivation film could be formed in the 6.0 wt.% FeCl3 solution. However, the chloride ion radius was very small, and it was easy to penetrate the passivation film, resulting in pitting corrosion, which limited the continuation of the passivation zone [27,28].
Figure 7. Higher magnification of the SEM images of the surface (a) and cross-section (b) of the SS316L SLM sample after anodic polarisation testing in a 6.0 wt.% FeCl3 solution at 25 °C and an EDS analysis of selected areas on the surface (c).
microstructure between the un-melted powder and the re-melted area, microcells were easily formed, and the re-melted areas were more susceptible to corrosion in the 6.0 wt.% FeCl3 solution, in which Fe3+ had stronger oxidizing properties. Moreover, sample corrosion was more likely to occur within the grain and micro cracks, which might be attributed to the larger specific surface area of the primary cracks and pore sites . Therefore, a greater number of micro cracks, un-melted powders and pores inside the sample led to a stronger corrosion tendency of the samples in the FeCl3 solution. Area 1 was located in the un-melted powder, area 2 was located at the corrosion surface, and area 3 was taken from the substrate of the SS316L SLM sample. Obviously, in comparison to the SS316L components, the Ni, Mo and Si contents in areas 1 and 2 evidently decreased, but the Cr and Mn contents increased remarkably. The contents of Ni and Mo in area 2 were significantly lower than those in areas 1 and 2, while the contents of Cr, Mn and C were significantly higher than those in areas 1 and 2. The Fe contents in areas 1, 2 and 3 were similar to those of the initial 316L state. It could be considered that the effect of Cr and Mn seemed to inhibit the activity of Fe, Mo and Ni intermediates and formed a barrier against pitting corrosion [31,32]. The cross-sectional SEM image of the SLM sample from the fine powder following corrosion testing in a 6.0 wt.% FeCl3 solution is shown in Figure 7b. The depth of the crack propagation was up to 29.3 μm, and fine spherical powder with particle diameters less than 5 μm inside the crack was observed.
3.2. Weight loss tests after immersion corrosion experiment
Figure 8. Weight loss plots for the SS316L SLM samples from fine powder, coarse powder and raw powder as a function of time in a 6.0 wt.% FeCl3 solution at 25 °C.
Figure 9. SEM images of the XY-plane (a), vertical bamboo structure (b), flat bamboo structure (c) of the SS316L SLM sample from fine powder and the XZ-plane (d) of the SS316L SLM sample from coarse powder after an immersion corrosion experiment in a 6.0 wt.% FeCl3 solution at 25 °C for 25 days.
Figure 10. EDS spectra of the selected area of the corrosion product of the SS316L SLM sample from coarse powder after immersing in a 6.0 wt.% FeCl3 solution at 25 °C for 25 days.
with the content of Mn (2.27 wt.%) in the original SS316L SLM sample, the content of Mn (4.84 wt.%) on the surface of the corroded sample was significantly increased, which further indicated that the element of Mn was more easily corroded to form corrosion products and was enriched on the surface of the sample. There was a little Cl on the surface of the sample, mainly because most of the chloride was dissolved into the solution . The presence of element Cl explained the process of Cl -penetration into the matrix through the oxide film.
As shown in Figure 11, the corrosion product phases from the SS316L SLM sample immersed in a 6.0 wt.% FeCl3 solution at 25 °C for 25 days were identified by X-ray diffraction pattern analyses . Various phases such as iron chloride hydrate [FeCl2•(H2O)4], chromium oxide [Cr2O3] and [CrO2], nickel iron oxide [NiFe2O4], nickel chromium oxide [NiCrO4], manganese oxide [Mn2O3], and molybdite [MoO3] phases were detected in the XRD patterns. The XRD pattern of the corrosion products that occurred after 25 days in the 6.0 wt.% FeCl3 solution illustrated that the FeCl2•(H2O)4 phase was the major corrosion product with smaller quantities of other oxides.
Figure 11. XRD patterns of the corrosion products of the SS316L SLM sample after immersing in a 6.0 wt.% FeCl3 solution at 25 °C for 25 days.
3.3. Corrosion mechanism
Figure 12 interprets the corrosion mechanisms of SS316L produced via SLM from different size powders in the 6.0 wt.% FeCl3 solution during the four stages . In the first instance, a stable passive layer was generated on the surface of the sample, pores, cracks and un-melted powders (Figure 12b).
attack and break through passivation membrane into the internal matrix to form pitting corrosion. For the rough surface (containing cracks, pores and un-melted powder), the Cl- first entered into the cracks and pores to facilitate crevice corrosion because of the high surface free energy of the cracks and pores . Meanwhile, due to the strong oxidation of Fe3+ in the solution, Fe was oxidized to Fe2+, Cr was oxidized to Cr3+ and Cr4+, Ni was oxidized to Ni2+, Mn as oxidized to Mn3+ and Mo was oxidized to Mo6+. In this study, Fe, Cr, Ni, Mn and Mo acted as the anodes. The reaction mechanism was shown in equations (1) - (5). The cathodic reaction must balance the dissolution reaction of the SS316L SLM sample substrate in the anode. The reduction of Fe3+ is the most dominant cathodic reaction that occurred, as shown in equation (6) .
Fe → Fe2+
+ 2e (1) Cr → Cr2+
+ 2e (2) Ni → Ni2+
+ 2e (3) Mn → Mn3+
+ 3e (4) Mo → Mo6+
+ 6e (5) Fe3+ + e → Fe2+ (6)
During Stage 3, as shown in Figure 12d, the corrosion products accumulated on the substrate surface, and the most of the corrosion products on the smooth surface fell off into the FeCl3 solution, so that the matrix was again exposed to the corrosion solution, repeating the process of Stage 2. The corrosion products on the rough surface were mostly enriched on the surface, and the vast majority of the corrosion products in the cracks were deposited and blocked the corrosion channels to prevent further corrosion.
In the end, the general disintegration of the corrosion products could be observed (Figure 12e).
Figure 12. Corrosion mechanisms of SS316L produced via SLM, stage 0: Initial stage (a), stage 1: passive layer is generated on the surface of the sample (b), stage 2: attack and breakage through the passivation membrane (c), stage 3: corrosion products fall off or are deposited on the surface (d), stage 4: further attack and breakage through the passivation membrane (e).
The microstructure, defects and corrosion characteristics of three SS316L SLM samples produced from three types of powder with different particle size distributions in a 6.0 wt.% FeCl3 solution were investigated. The following conclusions were drawn.
(1) SLM samples from the fine powder exhibited the best surface quality, which was smoother with less porosity and un-melted powder, while the SLM samples from coarse powder and raw powder possessed more pores and un-melted powders under the same SLM processing parameters.
(2) From the electrochemical polarization curves, the SLM sample from fine powder showed the lowest corrosion tendency, and the corrosion characteristics of the SLM sample from coarse powder was similar to that of the SLM sample from raw powder. The icorr and weight loss showed that the corrosion rate of the fine powder sample was the fastest.
(3) For the SS316L SLM sample, the Mn element was easily corroded and formed a corrosion product layer that acted like a barrier, while the Mo and Ni elements were more easily protected in the 6.0 wt.% FeCl3 solution.
The authors are grateful to the Research and Development Program of Sichuan Province (15ZC0370) for the financial support of this work.
1. H. Zhong, X. Yao, Y. Zhu, J. Zhang, D. Jiang, J. Chen, Z. Chen, X. Liu and Z. Huang, J. Ceram. Sci. Tech., 06 (2015) 133.
2. J.S. Park; M.G. Lee, Y.J. Cho, J.H. Sung, M.S. Jeong, S.K. Lee, Y.J. Choi and D.H. Kim, Met. Mater. Int., 22 (2016) 143.
3. Y. Zou, Q. Han, X.S. Weng, Y.W. Zou, Y.Y. Yang, K.S. Zhang, K.R. Yang, X.L. Xu, C.Y. Wang, Y.G. Qin and J.C. Wang, Medicine, 6 (2018) 97.
4. K.A. Ibrahim, B. Wu and N.P. Brandon, Mater. Design, 106 (2016) 51. 5. Z.J. Sun, X.P. Tan, S.B. Tor, W.Y. Yeong, Mater. Design, 104 (2016) 197.
6. A. Hinojos, J. Mireles, A. Reichardt, P. Frigola, P. Hosemann, L.E. Murr and R.B. Wicker, Mater. Design, 94 (2016) 17.
7. R.K. Enneti, K.C. Prough, T.A. Wolfe, A. Klein, N. Studley and J.L. Trasorras, Int. J. Refract. Met. H., 71 (2018) 28.
8. Y. Zhong, L.F. Liu, S. Wikman, D.Q. Cui and Z.J. Shen, J. Nucl. Mater., 470 (2016) 170. 9. K.V. Yang, Y.J. Shi, F. Palm, X.H. Wu and P. Rometsch, Scripta Mater., 145 (2018) 113. 10.K. Kunze, T. Etter, J. Grässlin and V. Shklover, Mater. Sci. Eng. A, 620 (2015) 213.
11.L.B. Zhou, T.C. Yuan, R.D. Li, J.Z. Tang, G.H. Wang and K.X. Guo, Mater. Sci. Eng. A, 707 (2017) 443.
12.S. Leuders, M. Thöne, A. Riemer, T. Niendorf, T. Tröster, H.A. Richard and H.J. Maier, Int. J. Fatigue, 48 (2013) 300.
13.Z.L. Lu, A.F. Zhang and Z.Q. Tong, Mater. Manuf. Process., 26 (2011) 879. 14.D.K. Pattanayak, A. Fukuda and T. Matsushita, Acta Biomater., 7 (2011) 1398. 15.Y. Sun, A. Moroz and K. Alrbaey, J. Mater. Eng. Perform., 23 (2014) 518.
18.E. Otero, A.A Pardo, M. V. Utrilla, E. Sáenz and J.F. Álvarez, Corros. Sci, 40 (1998) 1421. 19.D. Itzhak and E. Aghion, Corros. Sci., 23 (1983) 1085.
20.P. Nandwana, A.M. Elliott, D. Siddel, A. Merriman, W.H. Peter and S.S. Babu, Curr. Opin. Solid St. M., 21 (2017) 207.
21.P.P. Ding, A.Q. Mao, X. Zhang, X. Jin, B. Wang, M. Liu and X.L. Gu, J. Alloy. Compd., 721 (2017) 609.
22.A.Y. Chen, W.F. Hu, D. Wang, Y.K. Zhu, P. Wang, J.H. Yang, X.Y. Wang, J.F. Gu and J. Lu, Scripta Mater., 130 (2017) 264.
23.L.Y. Chen, J.C. Huang, C.H. Lin, C.T. Pan, S.Y. Chen, T.L. Yang, D.Y. Lin, H.K. Lin and J.S.C. Jang, Mater. Sci. Eng. A, 682 (2017) 389.
24.N.J. Harrison, I. Todd and K. Mumtaz, J. Mater. Sci., 52 (2017) 10517. 25.K. Sasaki and G.T. Burstein, Corros. Sci., 38 (1996) 2111.
26.G. Sander S. Thomas, V. Cruz, M. Jurg, N. Birbilis, X. Gao, M. Brameld and C.R. Hutchinson, J. Electrochem. Soc., 164 (2017) 250.
27.E. Mccafferty, Corros. Sci., 45 (2003) 1421. 28.J. Soltis, Corros. Sci., 90 (2015) 5.
29.A.B. Radwan, A.M. Abdullah, H.J. Roven, A.M. Mohamed and M.H. SK, Int. J. Electrochem. Sci., 10 (2015) 7606.
30.Q. Chao, V. Cruz, S. Thomas, N. Birbilis, P. Collins, A. Taylor, P.D. Hodgson and D. Fabijanic, Scripta Mater., 141 (2017) 94.
31.M. Bojinov, G. Fabricus, T. Laitinen, K. Mäkelä, T. Saario, G. Sundholm, Electrochim. Acta, 46 (2001) 1339.
32.W.Y. Lai, W.Z. Zhao, Z.F. Yin and J. Zhang, Surf. Interface Anal., 44 (2012) 505.
33.Y. Chen, J.X. Zhang, X.H. Gu, N.W. Dai, P. Qin and L.C. Zhang, J. Alloy. Compd., 747 (2018) 648. 34.M. Cabrini, S. Lorenzi, T. Pastore, S. Pellegrini, E.P. Ambrosio, F. Calignano, D. Manfredi, M.
Pavese and P. Fino, Electrochim. Acta, 206 (2016) 346.
35.K. Jung, H.J. Heo, J.H. Lee, Y.C. Park and C.Y. Kang, Corros. Sci., 98 (2015) 748. 36.M. Qin, W.C. Xu, L.H. Yang and Y.T. Li, Int. J. Electrochem. Sci., 13 (2018) 6537. 37.K.E. García, A.L. Morales, C.A. Barrero and J.M. Greneche, Corros. Sci., 48 (2006) 2813.
38.Y. Behnamian, A. Mostafaei, A. Kohandehghan, B. Zahiri, W.Y. Zheng, D. Guzonas, M. Chmielus, W.X. Chen and J.L. Luo, J. Supercrit. Fluid., 127 (2017) 191.
39.W.S.W. Harun, R.I.M. Asri, F.R.M. Romlay, S. Sharif, N.H.M. Jan and F. Tsumori, J. Alloy. Compd., 748 (2018) 1044.